Thermal properties of carbon black aqueous nanofluids for solar absorption
© Han et al; licensee Springer. 2011
Received: 19 March 2011
Accepted: 18 July 2011
Published: 18 July 2011
In this article, carbon black nanofluids were prepared by dispersing the pretreated carbon black powder into distilled water. The size and morphology of the nanoparticles were explored. The photothermal properties, optical properties, rheological behaviors, and thermal conductivities of the nanofluids were also investigated. The results showed that the nanofluids of high-volume fraction had better photothermal properties. Both carbon black powder and nanofluids had good absorption in the whole wavelength ranging from 200 to 2,500 nm. The nanofluids exhibited a shear thinning behavior. The shear viscosity increased with the increasing volume fraction and decreased with the increasing temperature at the same shear rate. The thermal conductivity of carbon black nanofluids increased with the increase of volume fraction and temperature. Carbon black nanofluids had good absorption ability of solar energy and can effectively enhance the solar absorption efficiency.
Keywordsnanofluids solar absorption carbon black photothermal properties rheological behaviors thermal conductivity
The major resource of renewable energy comes from the sun. Solar energy utilization is very important in the background of global warming and reduction of carbon dioxide emission. Solar energy has been explored through solar thermal utilization, photovoltaic power generation, and so on [1–3]. Solar thermal utilization is the most popular application among them. In conventional solar thermal collectors, plates or tubes coated with a layer of selectively absorbing material are used to absorb solar energy, and then energy is carried away by working fluids in the form of heat [4, 5]. This type of collector exhibits several shortcomings, such as limitations on incident flux density and relatively high heat losses . In order to overcome these drawbacks, direct solar absorption collector has been used for solar thermal utilization. In this kind of collector, solar energy is directly absorbed by the working fluids meanwhile the generated heat is carried out by the working fluids .
In the last century, black liquids containing millimeter to micrometer-sized particle were used as working fluid in solar collectors due to their excellent photothermal properties . However, the applications of these suspensions are limited because of severe abrasion, sedimentation, and plug problems of coarse particles. Recently, nanofluids have been applied as working fluids in direct solar collectors [5, 8–11]. Nanofluid is a new class of heat transfer fluids containing stably suspended nano-sized particles, fibers, or tubes in the conventional heat transfer fluids such as water, ethylene glycol, engine oil, etc. [12–16]. Several researchers have reported that nanofluids could effectively improve the solar energy utilization [4, 17, 18]. Taylor et al. found that nanofluids had excellent potential for solar thermal power plants. Efficiency improvement on the order of 5% to 10% was possible with a nanofluid receiver . Shin et al. reported that the specific heat of a high temperature nanofluid (1 wt.% silica nanoparticles in a eutectic of lithium carbonate and potassium carbonate) enhanced by 25% compared with that of the pure eutectic . The results of Tyagi et al. showed that the absolute efficiencies of the Al/water nanofluid-based direct absorption solar collectors were about 10% higher than that of the conventional flat-plate type collectors using pure water under similar operating conditions . Mu et al. investigated the radiative properties of SiO2/water, TiO2/water, and ZrC/water nanofluids. They found that the ZrC nanofluid had the highest solar absorbance among the studied nanofluids . However, the research on the solar energy utilization of nanofluids is only in the start stage, and the relative reports are scarce at present.
When nanofluids are used as working fluids of the direct solar absorbers, the thermal properties of nanofluids are critical to the solar utilization. Photothermal property is very important to the assessment of solar energy absorption of nanofluids because it directly reflects the solar absorption ability of nanofluids. Viscosity and rheological behaviors not only are essential parameters for nanofluid stability and flow behaviors but also affect the heat transfer efficiency of direct solar absorbers. Thermal conductivity is an important parameter for heat transfer fluids. It also affects the collectors' heat transfer efficiency. Great efforts have been made to the rheological behaviors and thermal conductivities of nanofluids [21–27], and these studies are helpful to the research of nanofluids as solar absorption working fluids. However, as mentioned above, there are only a few research committed to the photothermal properties [5, 18]. Therefore, more studies are essential to the photothermal property research.
Carbon black is a kind of material that has very good absorption in the whole wavelength range of sunlight . Carbon black nanofluids seem to have high potentials in the application of solar utilization. However, there are only a few researches on carbon black nanofluids [28–31], which mainly concern about the viscosity, dispersion stability, and tribological behavior.
In this study, carbon black nanofluids were prepared by dispersing the pretreated carbon black powder into distilled water. The size and morphology of the nanoparticles were explored. The photothermal properties, optical properties, rheological behaviors, and thermal conductivities of the nanofluids were also investigated.
Preparation of nanofluids
Commercial carbon black powder (N115) was supplied by Qingdao Degussa Company, Qingdao, China. To obtain stable nanofluids, the original carbon black powder was pretreated as follows: 15 g of original carbon black powder and 300 ml 30% H2O2 were added into a round-bottomed flask and heated to boiling under magnetic stirring. The reaction was carried out under stirring and boiling for 5 h. Then the mixture was filtrated at room temperature and dried at 100°C. Pretreated carbon black powder was obtained by repeating the process twice. Then the pretreated carbon black powder was ground and dispersed into distilled water under ultrasonic vibration for 1 h. Carbon black nanofluids of different particle volume fractions were prepared by adjusting the amount of carbon black and water.
Characterization of carbon black nanofluids
The transmission electron microscopy (TEM) images were captured on a JEM-2000EX (JEOL Ltd., Tokyo, Japan) transmission electron microscope with an acceleration voltage of 160 kV. The carbon black nanofluids were diluted with distilled water and one drop was placed on a carbon-coated copper grid and left to dry at room temperature. Particle size distributions of the nanoparticles in nanofluids were measured with a Zetasizer 3000HS (Malvern, Worcestershire, UK) particle size analyzer based on dynamic light scattering technology. The samples were also prepared by diluting the nanofluids with distilled water.
Measurements of photothermal properties of carbon black nanofluids
Measurements of optical properties of carbon black powder and nanofluids
UV-Vis-NIR spectra of pretreated carbon black powder and nanofluids were recorded on a CARY-500 spectrophotometer (MedWOW, Necosia, Cyprus) at room temperature from 200 to 2,500 nm. The carbon black powder was put on a sample stage, and the absorption spectra were detected. The carbon black nanofluids of different volume fraction were put into quartz cuvettes, and the transmittance spectra were detected.
Measurements of rheological behaviors of carbon black nanofluids
The rheological behaviors of the carbon black nanofluids were investigated on a controlled stress viscometer (Physica MCR301, Anton Paar, Graz, Austria) with a cylindrical rotor. The shear rate and temperature ranged from 15 to 110 s-1 and 25°C to 50°C, respectively. A continuous reading of shear stress and shear rate was recorded automatically when the measurement process was stabilized after the nanofluids were transferred into a measurement chamber. The cylindrical sample cell was surrounded with a constant temperature water bath. The temperature measurement accuracy was 0.01°C.
Measurements of thermal conductivity of carbon black nanofluids
The thermal conductivity was measured on a KD2 Pro Thermal Property Analyzer (Decagon Inc., Pullman, WA, USA) using a single-needle sensor for heating and monitoring of the temperature, which is based on the transient hot wire method. The instrument's probe (1.3 mm in diameter and 60-mm long) was vertically immersed in the center of nanofluids. The thermal conductivity range of the probe was 0.02 to approximately 2 Wm-1K-1. The dimensions of cylindrical sample cell were 35 mm in diameter and 70 mm in length. Each measurement took 1 min. Calibration of the probe was carried out first by measuring the thermal conductivity of pure water, ethylene glycol, and glycerol. All our measurements were performed over ten times and averaged, and the time interval between the measurements was 15 min.
Results and discussion
Characterization of typical sample
Photothermal properties of carbon black nanofluids
Optical properties of carbon black powder and nanofluids
Rheological behaviors of carbon black nanofluids
As the shear rate increases, the aggregation structures of the nanoparticles break down. As a result, the viscosity decreases, and shear thinning behaviors are observed. With the increase of the carbon black concentration, the interaction between the nanoparticles enhances, and the flow resisting force increases. Therefore, the viscosity and the heat resistance increase with the increase of the volume fraction.
With the increase of the temperature, Brownian motion enhances, and hence, the interaction between the nanoparticles decreases. The solvent effect of the carbon black particles also decreases at high temperatures. These might be responsible for the small viscosity at high temperatures. When the temperature goes up, the viscosity of the nanofluids decreases, and thus the flow resisting force and heat resistance decreases. This is helpful to improve the efficiency of the solar absorbers at high temperatures.
Thermal conductivity of carbon black nanofluids
When the volume fraction increases, the effective medium increases. As a result, the thermal conductivity increases with the volume fraction. As mentioned above, the solar adsorption ability also enhances with the volume fraction. However, as the concentration of carbon black increases, the viscosity and flow resisting force increases. Thus, the heat transfer efficiency decreases. Therefore, there should be an optimum volume fraction. Considering these thermal properties, the 6.6 vol.% carbon black nanofluids have better solar thermal utilization properties.
Carbon black nanofluids were prepared by dispersing the pretreated carbon black powder into distilled water. The nanofluids of high-volume fraction have better photothermal properties which indicate better solar energy adsorption properties. Both carbon black powder and nanofluids have good absorption in the whole wavelength range from 200 to 2,500 nm. The nanofluids exhibit a shear thinning behavior. The shear viscosity increases with the increasing volume fraction and decreases with the increasing temperature at the same shear rate. The thermal conductivity of carbon black nanofluids increases with the increase of volume fraction and temperature. In conclusion, carbon black nanofluids have good absorption ability of solar energy and can effectively enhance the solar absorption efficiency. As a result, carbon black nanofluids have high potentials for the application of solar utilization.
transmission electron microscopy.
The authors gratefully acknowledge the support of the Natural Science Foundation of Shandong Province (ZR2010EM035) and Qingdao Science and Technology Project (2010-3-4-4-12-jch).
- Duffie JA, Beckman WA: Solar Engineering of Thermal Processes. New York: John Wiley & Sons; 1980.Google Scholar
- Tripanagnostopoulos Y: Aspects and improvements of hybrid photovoltaic/thermal solar energy systems. Sol Energy 2007, 81: 1117–1131. 10.1016/j.solener.2007.04.002View ArticleGoogle Scholar
- Charalambous PG, Maidment GG, Kalogirou SA, Yiakoumetti K: Photovoltaic thermal (PV/T) collectors: A review. Appl Therm Eng 2007, 27: 275–286. 10.1016/j.applthermaleng.2006.06.007View ArticleGoogle Scholar
- Otanicar TP, Golden JS: Comparative environmental and economic analysis of conventional and nanofluid solar hot water technologies. Environ Sci Technol 2009, 43: 6082–6087. 10.1021/es900031jView ArticleGoogle Scholar
- Mu LJ, Zhu QZ, Si LL: Radiative properties of nanofluids and performance of a direct solar absorber using nanofluids. 2nd ASME Micro/Nanoscale Heat & Mass Transfer International Conference 2010, 1: 549–553.Google Scholar
- Tyagi H, Phelan P, Prasher R: Predicted efficiency of a low-temperature nanofluid-based direct absorption solar collector. J Sol Energy Eng 2009, 131: 041004. 10.1115/1.3197562View ArticleGoogle Scholar
- Minardi JE, Chuang HN: Performance of a black liquid flat-plate solar collector. Sol Energy 1975, 17: 179–183. 10.1016/0038-092X(75)90057-2View ArticleGoogle Scholar
- Bertocchi R, Karni J, Kribus A: Experimental evaluation of a non-isothermal high temperature solar particle receiver. Energy 2004, 29: 687–700. 10.1016/j.energy.2003.07.001View ArticleGoogle Scholar
- Otanicar TP, Phelan PE, Golden JS: Optical properties of liquids for direct absorption solar thermal energy systems. Sol Energy 2009, 83: 969–977. 10.1016/j.solener.2008.12.009View ArticleGoogle Scholar
- Shou CH, Luo ZY, Wang T, Cai JC, Zhao JF, Ni MJ, Cen KF: Research on the application of nano-fluids into the solar photoelectric utilization. Shanghai Electric Power 2009, 16: 8–12.Google Scholar
- Otanicar TP, Phelan PE, Prasher RS, Rosengarten G, Taylor RA: Nanofluid-based direct absorption solar collector. J Renewable and Sustainable Energy 2010, 2: 033102. 10.1063/1.3429737View ArticleGoogle Scholar
- Choi SUS: Enhancing thermal conductivity of fluids with nanoparticles. In Developments and Applications of Non-Newtonian Flows. Edited by: Singer DA, Wang HP. New York: American Society of Mechanical Engineers; 1995:99–105. FED 231/MD 66 FED 231/MD 66Google Scholar
- Das SK, Choi SUS, Yu W, Pradeep T: Nanofluids: Science and Technology. New Jersey: John Wiley & Sons; 2007.View ArticleGoogle Scholar
- Zhu HT, Liu SQ, Xu L, Zhang CY: Preparation, characterization and thermal properties of nanofluids. In Leading Edge Nanotechnology Research Developments. Edited by: Sabatini DM. New York: NOVA Science Publisher; 2008:5–38.Google Scholar
- Wu DX, Zhu HT, Wang LQ, Liu LM: Critical issues in nanofluids preparation, characterization and thermal conductivity. Current Nanoscience 2009, 5: 103–112. 10.2174/157341309787314548View ArticleGoogle Scholar
- Wang LQ, Fan J: Nanofluids research: key issues. Nanoscale Res Lett 2010, 5: 1241–1252. 10.1007/s11671-010-9638-6View ArticleGoogle Scholar
- Tyagi H, Phelan P, Prasher R: Predicted efficiency of a nanofluid-based direct absorption solar receiver. Proceedings of the Energy Sustainability Conference 2007 2007, 729–736.View ArticleGoogle Scholar
- Mao LB, Zhang RY, Ke XF: The photo-thermal properties of copper-nanofluids. Journal of Guangdong University of Technology 2008, 25: 13–17.Google Scholar
- Taylor RA, Phelan PE, Otanicar TP, Walker CA, Nguyen M, Trimble S, Prasher R: Applicability of nanofluids in high flux solar collectors. J Renewable and Sustainable Energy 2011, 3: 023104. 10.1063/1.3571565View ArticleGoogle Scholar
- Shin DH, Banerjee D: Enhanced specific heat of silica nanofluid. J Heat Trans-T ASME 2011, 133: 024501. 10.1115/1.4002600View ArticleGoogle Scholar
- Chen HS, Ding YL, Tan CQ: Rheological behaviour of nanofluids. New J Phys 2007, 9: 36701–36724.Google Scholar
- Chevalier J, Tillement O, Ayela F: Rheological properties of nanofluids flowing through microchannels. Appl Phys Lett 2007, 91: 233103. 10.1063/1.2821117View ArticleGoogle Scholar
- Schmidt AJ, Chiesa M, Torchinsky DH, Johnson JA, Boustani A, McKinley GH, Nelson KA, Chen G: Experimental investigation of nanofluid shear and longitudinal viscosities. Appl Phys Lett 2008, 92: 244107. 10.1063/1.2945799View ArticleGoogle Scholar
- Zhu HT, Li CJ, Wu DX, Zhang CY, Yin YS: Preparation, characterization, viscosity and thermal conductivity of CaCO 3 aqueous nanofluids. Science China-Technological Sciences 2010, 53: 360–368. 10.1007/s11431-010-0032-5View ArticleGoogle Scholar
- Jang SP, Hwang KS, Lee JH, Kim JH, Lee BH, Choi SUS: Effective thermal conductivities and viscosities of water-based nanofluids containing Al 2 O 3 with low concentration. 2007 7th IEEE Conference on Nanotechnology, Vol 1–3 2007, 1015–1018.Google Scholar
- Xie HQ, Yu W, Li Y, Chen LF: Influencing factors for thermal conductivity enhancement of nanofluids. 2nd ASME Micro/Nanoscale Heat & Mass Transfer International Conference 2010, 1: 591–598.Google Scholar
- Buongiorno J, Venerus DC, Prabhat N, McKrell T, Townsend J, Christianson R, Tolmachev YV, Keblinski P, Hu LW, Alvarado JL, Bang IC, Bishnoi SW, Bonetti M, Botz F, Cecere A, Chang Y, Chen G, Chen H, Chung SJ, Chyu MK, Das SK, Di Paola R, Ding Y, Dubois F, Dzido G, Eapen J, Escher W, Funfschilling D, Galand Q, et al.: A benchmark study on the thermal conductivity of nanofluids. J Appl Phys 2009, 106: 094312. 10.1063/1.3245330View ArticleGoogle Scholar
- Cheng B, Du K, Zhang XS, Yang L: Influence of ingredients of carbon black nano-particle suspension of ammonia solution on viscosity of nanofluid. J Hunan Univ 2009, 36: 115–119.Google Scholar
- Hwang Y, Lee JK, Jeong YM, Cheong SI, Ahn YC, Kim SH: Production and dispersion stability of nanoparticles in nanofluids. Powder Technol 2008, 186: 145–153. 10.1016/j.powtec.2007.11.020View ArticleGoogle Scholar
- Vander Wal RL, Mozes SD, Pushkarev V: Nanocarbon nanofluids: morphology and nanostructure comparisons. Nanotechnology 2009, 20: 105702. 10.1088/0957-4484/20/10/105702View ArticleGoogle Scholar
- Choi C, Jung M, Choi Y, Lee J, Oh J: Tribological properties of lubricating oil-based nanofluids with metal/carbon nanoparticles. J Nanosci Nanotechnol 2011, 11: 368–371. 10.1166/jnn.2011.3227View ArticleGoogle Scholar
- Tseng WJ, Lin KC: Rheology and colloidal structure of aqueous TiO 2 nanoparticle suspensions. Mat Sci Eng A-Struct 2003, 355: 186–192. 10.1016/S0921-5093(03)00063-7View ArticleGoogle Scholar
- Tamjid E, Guenther BH: Rheology and colloidal structure of silver nanoparticles dispersed in diethylene glycol. Powder Technol 2010, 197: 49–53. 10.1016/j.powtec.2009.08.022View ArticleGoogle Scholar
- Zhu HT, Han DX, Meng ZG, Wu DX, Zhang CY: Preparation and thermal conductivity of CuO nanofluid via a wet chemical method. Nanoscale Res Lett 2011, 6: 181. 10.1186/1556-276X-6-181View ArticleGoogle Scholar
- Shima PD, Philip J, Raj B: Influence of aggregation on thermal conductivity in stable and unstable nanofluids. Appl Phys Lett 2010, 97: 153113. 10.1063/1.3497280View ArticleGoogle Scholar
- Philip J, Shima PD, Raj B: Evidence for enhanced thermal conduction through percolating structures in nanofluids. Nanotechnology 2008, 19: 305706. 10.1088/0957-4484/19/30/305706View ArticleGoogle Scholar
- Das SK, Putra N, Thiesen P, Roetzel W: Temperature dependence of thermal conductivity enhancement for nanofluids. J Heat Trans-T ASME 2003, 125: 567–574. 10.1115/1.1571080View ArticleGoogle Scholar
- Li CH, Peterson GP: Experimental investigation of temperature and volume fraction variations on the effective thermal conductivity of nanoparticle suspensions (nanofluids). J Appl Phys 2006, 99: 084314. 10.1063/1.2191571View ArticleGoogle Scholar
- Chon CH, Kihm KD, Lee SP, Choi SUS: Empirical correlation finding the role of temperature and particle size for nanofluid (Al 2 O 3 ) thermal conductivity enhancement. Appl Phys Lett 2005, 87: 153107. 10.1063/1.2093936View ArticleGoogle Scholar
- Murshed SMS, Leong KC, Yang C: Investigations of thermal conductivity and viscosity of nanofluids. Int J Therm Sci 2008, 47: 560–568. 10.1016/j.ijthermalsci.2007.05.004View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.